Twolevel states in glasses


 Everett Fleming
 2 years ago
 Views:
Transcription
1 Rep. Prog. Phys. 50 (1987) Printed in the UK Twolevel states in glasses W A Phillips Cavendish Laboratory, University of Cambridge, Madingley Road, Cambridge CB3 OHE, UK Abstract This review covers a wide range of experimental and theoretical studies of twolevel or tunnelling states in glasses. Emphasis is on fundamental physics rather than a detailed comparison of experiment and theory. Sections cover the static and dynamic properties of tunnelling states, their contribution to thermal properties and their response to weak and strong electric and acoustic fields, both steady state and pulsed. A section on metallic glasses focuses on the importance of electron tunnellingstate interactions, and a final section illustrates approaches to a microscopic description by means of selected examples. This review was received in February /87/ IOP Publishing Ltd 1657
2 1658 W A Phillips Contents 1, Introduction 2. Tunnelling states 2.1. Static description 2.2. Dynamics 3. Thermal properties 3.1. Thermal conductivity 3.2. Heat capacity 3.3. Thermal expansion 3.4. Energy relaxation and irreversibility 4. Response to external fields 4.1. Weak fields 4.2. Strong fields 4.3. Relaxation 5. Pulse echo experiments 5.1. General theory 5.2. Echo experiments 5.3. Spectral diffusion 6. Metallic glasses 7. Microscopic descriptions of tunnelling states 7.1. Relation to specific defects 7.2. Microscopic modelling 7.3. General theories 7.4. suffix Acknowledgments References Page
3 Twolevel states in glasses Introduction One of the more unexpected results in solid state physics was provided by the first reliable measurements below 1 K of heat capacity C and thermal conductivity K in a number of glasses (Zeller and Pohl 1971). Beforehand it had been argued that because lowtemperature thermal properties are dominated by phonons (quantised lattice vibrations) of low frequency, and because in crystals these phonons can be described as longwavelength sound waves propagating through an elastic continuum, there should be little difference between glasses and crystals in this regime where the phonons are insensitive to microscopic structure. In fact, as shown in figures 1 and 2 for vitreous and crystalline silica, the heat capacity and thermal conductivity are radically different in the two materials. \ Vitreous silica \ \ \ \ T IKI Figure 1. The heat capacity C( T) of vitreous silica and crystalline quartz as a function of temperature T (Jones 1982, after Zeller and Pohl 1971), plotted as C/T3 against T The results in aquartz are typical of an insulating crystal. The heat capacity varies as T3 below 10 K, where T is the absolute temperature, as expected from the Debye theory. This theory predicts that in the longwavelength limit the density of phonon states g(w) varies quadratically with the phonon (angular) frequency w if the velocity of sound U, is constant so that wq = v,,, where q is the phonon wavevector. At higher temperatures phonon dispersion initially gives a more rapid increase of g(w) with w, and so C increases more rapidly than T3, but ultimately, above the Debye temperature 0, C approaches the classical limit. The cubic temperature variation of K can be interpreted qualitatively by means of the kinetic formula K =fcv,l (1.1)
4 1660 W A Phillips 102 IO lo T ik1 Figure 2. The thermal conductivity K(T) of vitreous silica and crystalline quartz (Jones 1982, after Zeller and Pohl 1971), plotted logarithmically. where 1 is the phonon mean free path. At low temperatures phonons are scattered by defects in the crystal or by the surfaces of the sample, so that 1 is independent of temperature and K is therefore proportional to T3. Above 40 K the reduction of 1 by phononphonon scattering leads to the peak and subsequent fall in K. These ideas are well known and serve to emphasise the peculiarity of the results in vitreous silica, where C varies approximately as T and at 0.1 K is about two orders of magnitude greater in the glass than in the crystal. Below 1 K K varies as T19 but varies only slightly with temperature between 4 and 20 K before increasing at high temperatures to a value approaching that of crystalline quartz. Similar results are seen in a wide range of other amorphous solids; oxide, chalcogenide, elemental, polymeric and metallic glasses all show the same behaviour. A representative sample is shown in figures 3 and 4. The universality of the phenomena and the idealised temperature dependences of C proportional to T and K proportional to T proved great attractions for theorists. In retrospect this idealisation can be seen to have handicapped the search for a theoretical explanation, suggesting as it did very general models which were not supported by a detailed examination of the experimental results and which were ultimately unable to give quantitative agreement with experiment. For example, the first and perhaps most obvious explanation for C was in terms of electron states (Redfield 1971). In the amorphous state the sharp distinction between energy gaps
5 Twolevel states in glasses I I I I T2 ikz) Figure 3. C( T)/ T plotted as a function of T2 for a range of glasses (Stephens 1973). and energy bands can be blurred by disorder, and it was suggested that the specific heat was a result of an almost constant density of states at the Fermi level, giving a linear variation of C with T just as in a metal. However, it turns out that the density of states estimated from optical experiments (less than J' m3 or lo'* ev' cm') is much smaller than that deduced from the heat capacity ( J' m')). Similar quantitative problems arise in a model for thermal conductivity based on the scattering of sound waves by inhomogeneities in the glass structure, a form of Rayleigh scattering by variations in the local velocity of sound. In this case the magnitude of density fluctuations estimated thermodynamically or from light scattering experiments is too small to give significant scattering below 1 K, and although there is no independent way of directly estimating the local variation in velocity, the required magnitude is unreasonably large (Jones e? a1 1978). Sound waves are known to exist in glasses. In addition to measurements of the velocity of sound, limited to frequencies below about 1 GHz, evidence for the existence of well defined transverse and longitudinal waves comes from Brillouin scattering below 30 GHz (Vacher and Pelous 1976) and phonon interference experiments (Rothenfusser et a1 1983) up to 500GHz in vitreous silica. Consistent velocities are
6 1662 W A Phillips Figure 4. K( T) as a function of temperature for a range of glasses (Stephens 1973). measured in all these experiments, and the phonon mean free path is much greater than the wavelength. Further evidence is provided by measurements of thermal conductivity in very thin glass rods which have roughened surfaces to ensure that boundary scattering dominates (Pohl er a1 1974, Zaitlin and Anderson 1975). Experimental values agree with those calculated assuming the existence of sound waves. It is clear, therefore, that the unexpected thermal properties arise from additional excitations which both scatter phonons and contribute to the heat capacity. Of the various models originally proposed to account for the thermal data, the one most widely and successfully used has been the tunnelling or twolevelsystem model (Phillips 1972, Anderson et a1 1972). In this model, to be described in detail in the next section, atoms occupying one of two adjacent minima are assumed to tunnel quantum mechanically to the other, leading to a splitting of the ground state as in the ammonia molecule. The inevitable variations in local environment present in the amorphous solid give rise to a distribution of these splittings which is almost constant in energy, and hence to a heat capacity which can be evaluated as I: C(T) = n0(e2/4kbt2) sech2(e/2kbt) de (12) where no is the constant density of states and the other factor in the integrand is the contribution of a single twolevel state (Schottky anomaly). Evaluating the integral gives C(T)=(~ /6)nokg~T (1.3)
7 Twolevel states in glasses 1663 in broad agreement with experiment. These states scatter phonons, leading to a thermal conductivity proportional to T2 and to an acoustic attenuation which can be saturated at high acoustic intensities. It is this last property that provides the strongest evidence for the model which will form the basis for the interpretation of the wide range of experimental results discussed in this review. To a large extent the model can be used in phenomenological form, and possible microscopic representations will be described only in the last section. This review is not intended as a detailed evaluation and comparison of experimental results in specific glasses, but as a critical description of the way in which the tunnelling or twolevelsystem model can be used to explain a wide range of data. By far the largest number of experiments have been performed on vitreous silica, and this material will be used as a running example, although reference will be made to other materials when necessary. 2. Tunnelling states 2.1. Static description In a perfect crystal each atom is constrained by symmetry to occupy a single potential minimum. Many defects, however, can be represented microscopically as interstitial or substitutional impurity atoms or molecules moving in a multiminima potential provided by the neighbours. Such states have been extensively studied in, for example, alkali halides (Narayanamurti and Pohl 1970). At low temperatures a quantum mechanical description is necessary, and tunnelling of the atom from one minimum to another gives rise to the very small energy splittings (less than ev) needed if the states are to be observed in thermal experiments at 1 K and below. The tunnelling model proposes that similar states are intrinsic to glasses: an atom or group of atoms can occupy one of two (or more) potential minima. This choice at the microscopic level is consistent with the experimentally determined excess entropy of the glass with respect to the crystal, although the number of atoms contributing at low temperatures is only a small fraction of the total. The remainder are essentially immobile below the glasstransition temperature Tg. Each tunnelling state (TS) can be represented by a particle in a potential of the form shown in figure 5(a), where the abscissa may represent the position of one atom but more generally is a configurational coordinate describing a combination of the coordinates of a number of atoms. The energy levels of the particle are conveniently calculated using as a starting point the solutions of the singlewell problem, a choice of basis set 41 and d2 known as the well, nondiagonal or localised representation (figure S(b)). Each state is the ground state of the appropriate potential Vl or V, (assumed harmonic in figure 5). The complete Hamiltonian H can be written as H = HI + ( v  v, ) = Hz + ( v  V2) (2.1) where HI and H2 are the individual well Hamiltonians. In the localised representation the Hamiltonian matrix becomes If the extension of each localised wavefunction into the barrier is small, the terms (4il V V,14i) can be neglected in comparison to Ei, and if the zero of energy is chosen
8 1664 W A Phillips Figure 5. A doublewell potential (a), together with the wavefunctions in the localised (b) and diagonal (c) representations. as the mean of E, and E*, (2.2) becomes where the tunnel splitting A, is given by (2.3) A,= 2{4llf442)* (2.4) Notice that only if the wells are identical, apart from a relative shift in energy, is the A of (2.3) identical to that of figure 5(a). A, can be evaluated for specific potentials: two overlapping harmonic potentials in two and three dimensions (Mertzbacker 1970, Phillips 1981b) and Mathieu s equation for a rigid rotator in twofold and threefold potentials (Isnard and Gilchrist 1981) are typical examples. The results all imply a similar exponential dependence of A, on the barrier height and well separation, although precise numerical values change from one model to another. The use of a particular detailed form cannot be justified in amorphous solids (as opposed to crystals) because the microscopic picture is uncertain, and so a simplified expression is usually adequate: A,= hr ea = ha exp[d(2mv,/h2) *] (2.5) where hr is approximately equal to (E, + E2)/2, d is the separation and V, the barrier between the two wells, and m is the particle mass. Typical values of the tunnelling parameter A can be estimated from the requirement that A, must be approximately equal to kbt if the tunnelling state is to contribute to
9 Twolevel states in glasses 1665 thermal properties at a temperature T. At 1 K this requires a tunnel splitting of ev, which with hr equal to ev gives approximately 5 for A. This is equivalent to a bare proton tunnelling across a barrier of 0.1 ev with d = 0.7 A. The matrix (2.3) can be diagonalized to obtain the eigenstates, the true, diagonal or energy representation. These eigenfunctions, illustrated in figure 5, have energies *El2 where E =(A2+A~)1 2 (2.6) and can be written in the analytic forms 9, = cos 0+42 sin 0 (2.7) ~2=~1sinO~,cos0 (2.8) where tan 20=A,/A. In the symmetric case where A=O these equations give the expected symmetric and antisymmetric solutions. The I dipole moment of the tunnelling state can be written in terms of G1 and I,!J2 as PI = 9Tqx*1 dx = q [ (4Tx41 cos 0 + 4Tx4, sin2 O+ 47~4~ sin 20) dx if the term involving 4Tx42 can be neglected, and where po is the dipole moment when the particle is located in one well: po = [ I 4Tx4, dx =  4$x42 dx. Obviously p1 is zero for the symmetric case. For this, as for any problem involving two energy levels, there is a formal analogy with the problem of a spin; particle in a magnetic field. The Hamiltonian matrix (2.3) can therefore be rewritten in terms of the Pauli spin matrices (2.10) (or equivalently in terms of the spin operators S, =+ha,). After diagonalisation, the Hamiltonian takes the obvious form H =$EuZ. This analogy has important advantages when discussing nonlinear and coherent effects in the interaction of tunnelling states with acoustic and electric fields ( 5). A basic feature of the tunnelling state model as applied to amorphous solids is the existence of a wide range of values of both the tunnelling parameter A and the asymmetry A. Calculated properties of the states will depend critically on the form of the distribution function f(a, A,) for A and Ao, the latter distribution derived from that for A. In the case of the asymmetry A it is argued that the distribution function must be symmetric because both positive and negative values of A are equally likely. (No singularities are expected for A = 0 because the eigenstates remain nondegenerate.) The scale of energy variation is determined by the thermal energy available at the
10 1666 W A Phillips glasstransition temperature where the fluctuating local potentials of the liquid are frozen in the structure, Since Tg is between 200 and 1OOOK for most glasses, this energy is of the order of 0.05 ev, much larger than the thermal energy available at 1 K. The low temperature properties are therefore sensitive to the centre of a broad symmetric distribution, so that f(a, A,) can be taken as independent of A. The variation with A, is likely to be sensitive to the particular microscopic motion involved, although the general form can be deduced from the distribution of the tunnelling parameter A. Because of the exponential dependence of A, on A, only a relatively small range of A is sampled for a large range of A, and over this limited range the distribution of A can be assumed constant. The resulting distribution function can then be written f(a, A,) = P/AO. (2.11) This general result is only slightly modified (by a logarithmic factor) if the distribution of A varies slowly with the energy, but in general the precise dependence on A. will vary from one material to another, and can be regarded as a parameter to be determined by experiment (Frossatti et a1 1977, Phillips 1981b). The density of states n(e) can be calculated from (2.6) and the distribution function f(a, A,) only if a lower cutoff value for A, is introduced when integrating (2.11). Such a cutoff could arise from a maximum tunnelling parameter (Lasjaunias et a1 1978) or from characteristic time scales introduced by experiment. More precisely, the two parameters A and A. describing the states must be replaced by a second pair of parameters, often chosen as the energy E and the relaxation time T. The resulting distribution function for E and T will be derived in 0 3. In many cases the results of experiment can be interpreted and related in terms of a simpler model which ignores the detailed origin of the two levels. Instead, of two parameters A and A,, this twolevelsystem model considers the total energy E as the only variable. The distribution function is assumed to be constant. Although in many cases it is clear that the twolevelsystem model is inadequate for detailed understanding, in others the simplification introduced by its use is very helpful Dynamics The behaviour of a tunnelling state is defined by specifying the complex amplitudes a,(t) and a,(t) of the two lowest states with eigenfunctions $,(r) and $*(r). Neglect of higher states is justified because these two states are much closer in energy to each other than they are to other excited states, although the possibility that higher energy states might be important must be considered in certain cases (such as transition rates at temperatures above 1 K). The general timedependent wavefunction takes the form V(r, t) =a,(t)$l(r) exp(ie,t/a)+a,(t)$,(r) exp(ie,t/h) (2.12) where E, and E2 are the energies of states $, and $z and for normalisation alat+ a2at = 1. The complex nature of a, and a2 means that two quantities are necessary to define the twolevel system, normally taken as the difference in probabilities of finding the system in the two states, a2a~a,u~, and a quantity related to the phase difference between a, and a2, ala$. Measurable properties of the system depend on these two parameters, as can be seen for example by calculating the timedependent dipole
11 Twolevel states in glasses 1667 moment of a onedimensional tunnelling state. Using p, = p2 = ( $,IX~$~) and p12 = p2, = ($llx[i,b2), the average dipole moment (p( t)) can be written where hwo = E2  E,. Variations of a,( t) and a2( t) are determined through the timedependent Schrodinger equation by interaction with external fields. Any twolevel system in a solid will be subject to randomly varying strain fields which can be treated as the superposition of independent phonon modes. The strain field of each is weak, and interaction with the two levels can be treated using perturbation theory, ignoring phase coherence, equivalent to the interaction of an atom with electromagnetic radiation in a blackbody cavity (Phillips 1981b). Experimentally the properties of the states may be probed by strong external applied electromagnetic or strain fields where coherence of the two wavefunctions I,bl and I,b2 must be taken into account, although for weak external fields perturbation theory can still be used. Two related simplifications can be made. The frequency needed to induce resonant transitions from one level to the other is less than 20GHz for states contributing to thermal properties below 1 K. Corresponding wavelengths are 10 mm for photons and 100 nm for acoustic phonons, in both cases much larger than the spatial extent of the tunnelling or twolevel state. The dipole approximation, where the local electric or strain field is taken as uniform, is therefore valid. The dominant effect of these uniform fields is to affect the energy of the tunnelling state by changing the asymmetry energy, and changes in the barrier height can usually be ignored (Phillips 1981b, Anderson 1986). Any external perturbation is therefore diagonal in the local representation ( 41, &) which when transformed into the diagonal representation ( $1, $2) has the form cos24 sin24 l : : l sin24 cos24 In terms of the Pauli matrices the general interaction Hamiltonian can be written Hint= uz+ux l : : l (2.14) po*&+ uz+ux ye (2.15) in the presence of an electric field 5 and a strain field e. The two parameters po and y, defined as fda/dg and ;aa/ae respectively, are equivalent to the electric and elastic dipole moments of the equivalent classical problem of a charged particle moving in the double well potential. In (2.15) the vector character of is preserved, but the tensorial nature of e has been ignored and ye written as an average over orientations. For the twolevelsystem model (2.15) must be replaced by an equivalent form for Hint in which the relationship between the diagonal (uz) and offdiagonal (ux) terms is ignored. In this model (2.15) is usually written Hint= (t~u,+~ ux)5+(tduz+mux)e. (2.16) In the remainder of this section the phase coherence of I,b, and I,b2 will be ignored in a calculation valid for interaction with thermal phonons and weak external fields. The only relevant parameter is therefore the occupation probability p, = alar, with p1 +p2 = 1. Using a rateequation approach (Golding and Graebner 1981) P1= PIwl2+P2w2I (2.17) li2 =PIw12p2~12 (2.18)
12 1668 W A Phillips where wi2 is the transition probability from state 1 to state 2. In thermal equilibrium at temperature T, p1 and p2 are time independent, with values py and p:, so that where P h 2 = P b21 p:lp?= exp(elkt) = wi2lw2, (2.19) if E is the energy difference between the two levels. Replacing p2 in (2.17) gives $1 = PI(Wlr+ w21) + U 21 (2.20) defining a relaxation time T, where 1 T =(w12+w21)=w,2[1+exp (ElkT)]. (2.21) This relaxation time refers to the occupation probabilities, and so governs the relaxation of the term ala?  a2a; in the expression for (p) in (2.13). To distinguish it from the relaxation time for terms of the form ala: (see 0 4.2) it is often referred to as TI, or the spinlattice relaxation time. The transition probability can be calculated for a weak strain field using timedependent perturbation theory to give (2.22) where nb, the Bose factor, is [exp(e/kt)  l]', g(e) is the phonon density of states, and the summation is over phonon polarisations a. For an acoustic wave 2e, cos of the strain amplitude per phonon is given by equating the time average classical energy per unit volume to the energy of a phonon: 2pu2w2 = ho where U is the displacement amplitude and p is the bulk density. The strain is given by (2.23) where qa is the phonon wavevector, and the matrix element, using the term in ax in Hint (a, gives nothing), becomes 1/2 The Debye density of phonon states, valid in this lowenergy limit, is (2.24) g(e) = E2/2.rr2h3vi (2.25) per unit volume, where U, is the sound velocity for polarisation a. Collecting together (2.21), (2.22) and (2.24) gives (2.26) In the equivalent result for the twolevel system Ai is replaced by E', but it should be noted that this removes the very wide range of relaxation times predicted by (2.26) through the broad distribution of A,, and found experimentally ( At higher temperatures additional higherorder processes will of course contribute 1 o relaxation, but these have not been clearly observed in glasses.
13 3. Thermal properties 3.1. Thermal conductivity Twolevel states in glasses 1669 The interaction between TS and phonons reduces the phonon mean free path, and is the dominant scattering mechanism in glasses below 1 K. An expression for the free path, valid for weak fields (see 4) can be obtained from the rate equations, (2.17) and (2.18), using detailed balance between energy absorbed by the TS~ and energy lost by the phonons. For a single TS of energy E g(e)fipti=p1. Using (2.20) and (2.22) this can be written as defining a phonon scattering rate (3.2)  77y2,w A' tanh (E/k,T) pv: E2 (3.3) for the scattering of phonons of polarisation a by a single state with energy E and tunnel splitting A,. The total scattering at energy E is obtained by integrating over A. using f(a, A,) = PIA, (2.11) (noting that both +A and A contribute at a given E) which gives for the free path of a phonon of angular frequency w and polarisation cy. The thermal conductivity K( T) is evaluated on the assumption that heat is carried by nondispersive sound waves, consistent with the calculations leading to (2.26) and (3.4), and that scattering from TS dominates to give This gives general agreement with Lhe experimental results below 1 K both in respect of temperature dependence and magnitude, using the constant density of states derived from the heat capacity and a coupling constant y of order 1 ev. A more precise quantitative analysis requires information from acoustic experiments to separate longitudinal and transverse polarisation contributions in (3.6), and a more careful analysis of the heat capacity. Notice, however, that the interaction with phonons is dominated by TS with small asymmetry.
14 1670 W A Phillips Experimentally the temperature dependence is found to range from to T.9 indicating that the distribution function (2.11) is not strictly accurate. Eilack (1978) has pointed out that a distribution function of the form P(h) = P eua leads to K( T) proportional to TZPa, suggesting a width to the A distribution in the range This is not unreasonable, but the relatively small change in temperature depenldence shows the insensitivity of the calculation of K ( T) to the detailed form of the distribution functions. At higher temperatures the thermal conductivity passes through a plateau at temperatures between 4 and 20 K which has been explained in terms of increased scattering from a quadratically increasing density of TS (Zaitlin and Anderson 1975). Although there is some evidence from highfrequency acoustic measurements that the density of states may increase at higher energies (Pelous and Vacher 1976), it is extremely difficult to identify this contribution in the presence of relaxation scattering from the TS (3 4), higherorder phonon processes, structure scattering or even effects of phonon localisation Heat capacity The energy E and relaxation time T are more convenient parameters than A and A, when discussing heat capacity and other physical consequences of the distribution of tunnelling states. A distribution function (E, T) can be related to f(a, A,) by the Jacobian transformation This is a general result, but making use of the specific form f(a, A,) = P/Ao, D where P is the same constant that appears in 1;; (3.4) and T,~~(E), defined by replacing A, by E in (2.26), is the shortest relaxation time for states of energy E. The density of states is then given by integrating over all relaxation times from T, ~ up ~ to a value equal to the time scale to of the experiment: = $P ln(4t,/~,~~). The heat capacity can be calculated as in (1.1) to give m ~(t,) =;P 1n(4t,/~,,,) lo $$ sech ( ) 2kBT de (3.9) = &,rr2pkit ln(4t,/~,,,) (3.10) where the small energy variation of the logarithmic term, in the narrow range of E close to kbt which dominates the integral, has been neglected. Equation (3.10) encapsulates the nonequilibrium (nonergodic) nature of amorphous solids and not surprisingly has been the subject of numerous experimental
15 I I Twolevel states in glasses 1671 studies. Before examining the results on short time scales, it is helpful to assess the accuracy of (3.10) in respect of 'normal' measurements, where to is typically 10 s. Figure 6 shows C(T) in three samples of vitreous silica, Spectrosil B (about 1200ppm water), Suprasil (1000ppm water) and Suprasil W (almost no water). We will concentrate here on Suprasil W, where C( T) varies as T' in the range 25 mk < T < 250 mk, and where P = 3 x J' m3, yi = 1.6 ev and 7, = 1 ev can be deduced from K(T) and phonon echo experiments ( 3.1 and 5). The contribution of these states to C at 0.1 K can be calculated from (3.10) as 0.35 J kg' K' (taking to= 10 s and evaluating T,,, as 1 ps) in comparison to the experimental value of 0.7 J kg' K'. The logarithmic factor varies by 1.6 between 25 and 250 mk, giving a temperature variation approximately proportional to T' '. Bearing in mind a possible small energy dependence of P, the predicted temperature variation of C is in good agreement with experiment, although the magnitude is too small by a factor of two (Black 1978). This discrepancy could be ascribed to experimental uncertainties in the determination of yi and y, were it not for experiments at short time scales, which provide additional evidence that the reality is more complicated than that described by a single set of TS distributed according to (3.9). Such experiments are, however, notoriously Y  m m L al  h L. I I I I I I I 1 l l l l T IKI Figure 6. The heat capacity of 'waterfree' and 'wet' vitreous silica down to 25 mk. Also shown as a broken line is the Debye phonon contribution calculated from the velocities of sound (Lasjaunias et a[ 1975). 0, 0, Suprasil W (<1.5 ppmoh); 0, Suprasil (1200 ppm OH); A, Spectrosil B (1000 ppm OH) (Zeller and Pohl 1971).
16 1672 W A Phillips difficult (Goubau and Tait 1975, Kummer et a/ 1978, Lewis et a1 1978, Loponen et a/ 1980, 1982, Meissner and Spitzmann 1981). In general a short time scale is achieved by using thin samples of glass; at 0.4 K a sample 0.1 mm thick has a diffusion time of typically a few j ~ s. With a thin film heater on one side and a thermometer on the other the propagation of heat pulses through the sample can be followed to give either the diffusivity by fitting a diffusion equation to the measured temperature profile or the heat capacity by measuring the maximum temperature rise. One problem with this experimental arrangement is that even very thin metal films used as heaters or thermometers can have heat capacities comparable with the glass sample so that modelling thermal diffusion becomes difficult. There is limited agreement between the various experiments. Although all claim to see a timedependent heat capacity, the size of the effect differs greatly from one experiment to the next. The most consistent results are those of Meissner and Spitzmann (1981) (figure 7) and Loponen et a1 (1982) on Suprasil W, where the results tend to that predicted by (3.10) at time scales below 100 ps at temperatures below 1 K. For longer time scales C( t) changes more rapidly than expected, indicating another contribution to the heat capacity with a relatively well defined minimum relaxation time of about 100 ps at 0.3 K, and which when added to that derived from P gives approximate agreement with long time scale experiments below 1 K i Is) Figure 7. The measured heat capacity of vitreous silica as a function of the time scale of measurement at different temperatures: B 0.4 K; C, 0.6 K; E, 0.89 K; F, 1.0 K. The open circles represent the longtime data, and the broken lines the total heat capacity predicted by the tunnelling model. (Adapted from Meissner and Spitzmann (1981 ).)
Physics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More information5.6 Isobaric thermal expansion and isothermal compression (Hiroshi Matsuoka)
5.6 Isobaric thermal expansion and isothermal compression Hiroshi Matsuoka 1 5.6.2 he coefficient of thermal expansion as a response function to a temperature change he coefficient of thermal expansion
More informationConcept 2. A. Description of lightmatter interaction B. Quantitatities in spectroscopy
Concept 2 A. Description of lightmatter interaction B. Quantitatities in spectroscopy Dipole approximation Rabi oscillations Einstein kinetics in twolevel system B. Absorption: quantitative description
More informationFree Electron Fermi Gas (Kittel Ch. 6)
Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals  they are the glue that hold the nuclei together Types of binding (see next slide)
More informationLecture 3: Electron statistics in a solid
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
More informationNuclear Magnetic Resonance
Nuclear Magnetic Resonance Introduction Atomic magnetism Nuclear magnetic resonance refers to the behaviour of atomic nuclei in the presence of a magnetic field. The first principle required to understand
More informationWe consider a hydrogen atom in the ground state in the uniform electric field
Lecture 13 Page 1 Lectures 1314 Hydrogen atom in electric field. Quadratic Stark effect. Atomic polarizability. Emission and Absorption of Electromagnetic Radiation by Atoms Transition probabilities and
More informationDiamagnetism and Paramagnetism. Magnetization M(H) in the presence of an uniform magnetic field H at T=0 is defined as:
Diamagnetism and Paramagnetism Definitions: Magnetization M(H) in the presence of an uniform magnetic field H at T=0 is defined as: where is the ground state energy. Note that H is the magnetic field felt
More informationEnergy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)
Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact
More information particle with kinetic energy E strikes a barrier with height U 0 > E and width L.  classically the particle cannot overcome the barrier
Tunnel Effect:  particle with kinetic energy E strikes a barrier with height U 0 > E and width L  classically the particle cannot overcome the barrier  quantum mechanically the particle can penetrated
More informationPhysics 53. Wave Motion 1
Physics 53 Wave Motion 1 It's just a job. Grass grows, waves pound the sand, I beat people up. Muhammad Ali Overview To transport energy, momentum or angular momentum from one place to another, one can
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationChapter 9. Gamma Decay
Chapter 9 Gamma Decay As we have seen γdecay is often observed in conjunction with α or βdecay when the daughter nucleus is formed in an excited state and then makes one or more transitions to its ground
More informationChapter 8 Molecules. Some molecular bonds involve sharing of electrons between atoms. These are covalent bonds.
Chapter 8 Molecules (We have only three days for chapter 8!) 8.1 The Molecular Bond A molecule is an electrically neutral group of atoms held together strongly enough to behave as a single particle. A
More informationRate Equations and Detailed Balance
Rate Equations and Detailed Balance Initial question: Last time we mentioned astrophysical masers. Why can they exist spontaneously? Could there be astrophysical lasers, i.e., ones that emit in the optical?
More information thus, the total number of atoms per second that absorb a photon is
Stimulated Emission of Radiation  stimulated emission is referring to the emission of radiation (a photon) from one quantum system at its transition frequency induced by the presence of other photons
More informationIndiana's Academic Standards 2010 ICP Indiana's Academic Standards 2016 ICP. map) that describe the relationship acceleration, velocity and distance.
.1.1 Measure the motion of objects to understand.1.1 Develop graphical, the relationships among distance, velocity and mathematical, and pictorial acceleration. Develop deeper understanding through representations
More informationLecture 2: Semiconductors: Introduction
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
More informationMCEN Fall 2003.
Basic types of solid materials. Overview The theory of bands provides a basis for understanding the classification and physical properties of solid materials such as electrical conductivity, optical behavior
More information the total energy of the system is found by summing up (integrating) over all particles n(ε) at different energies ε
Average Particle Energy in an Ideal Gas  the total energy of the system is found by summing up (integrating) over all particles n(ε) at different energies ε  with the integral  we find  note:  the
More informationLecture 8: Extrinsic semiconductors  mobility
Lecture 8: Extrinsic semiconductors  mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............
More informationDynamics. Figure 1: Dynamics used to generate an exemplar of the letter A. To generate
Dynamics Any physical system, such as neurons or muscles, will not respond instantaneously in time but will have a timevarying response termed the dynamics. The dynamics of neurons are an inevitable constraint
More informationThis is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th
More informationLecture 18 Timedependent perturbation theory
Lecture 18 Timedependent perturbation theory Timedependent perturbation theory So far, we have focused on quantum mechanics of systems described by Hamiltonians that are timeindependent. In such cases,
More informationA wave lab inside a coaxial cable
INSTITUTE OF PHYSICS PUBLISHING Eur. J. Phys. 25 (2004) 581 591 EUROPEAN JOURNAL OF PHYSICS PII: S01430807(04)76273X A wave lab inside a coaxial cable JoãoMSerra,MiguelCBrito,JMaiaAlves and A M Vallera
More information in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons
Free Electrons in a Metal  in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons  if these electrons would behave like an ideal gas
More informationFIBER OPTICS. Prof. R.K. Shevgaonkar. Department of Electrical Engineering. Indian Institute of Technology, Bombay. Lecture: 09
FIBER OPTICS Prof. R.K. Shevgaonkar Department of Electrical Engineering Indian Institute of Technology, Bombay Lecture: 09 Analysis of Signal Distortion in Optical Fiber Fiber Optics, Prof. R.K. Shevgaonkar,
More informationThe First Law of Thermodynamics: Closed Systems. Heat Transfer
The First Law of Thermodynamics: Closed Systems The first law of thermodynamics can be simply stated as follows: during an interaction between a system and its surroundings, the amount of energy gained
More informationChapter 18 Statistical mechanics of classical systems
Chapter 18 Statistical mechanics of classical systems 18.1 The classical canonical partition function When quantum effects are not significant, we can approximate the behavior of a system using a classical
More informationThe Quantum Harmonic Oscillator Stephen Webb
The Quantum Harmonic Oscillator Stephen Webb The Importance of the Harmonic Oscillator The quantum harmonic oscillator holds a unique importance in quantum mechanics, as it is both one of the few problems
More informationAcoustic Velocity, Impedance, Reflection, Transmission, Attenuation, and Acoustic Etalons
Acoustic Velocity, Impedance, Reflection, Transmission, Attenuation, and Acoustic Etalons Acoustic Velocity The equation of motion in a solid is (1) T = ρ 2 u t 2 (1) where T is the stress tensor, ρ is
More informationDoes Quantum Mechanics Make Sense? Size
Does Quantum Mechanics Make Sense? Some relatively simple concepts show why the answer is yes. Size Classical Mechanics Quantum Mechanics Relative Absolute What does relative vs. absolute size mean? Why
More informationMicroscale and Nanoscale Heat Transfer
Sebastian Volz (Ed.) Microscale and Nanoscale Heat Transfer With 144 Figures and 7 Tables In Collaboration with Remi Carminati, Patrice Chantrenne, Stefan Dilhaire, Severine Gomez, Nathalie Trannoy, and
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationLaserinduced surface phonons and their excitation of nanostructures
CHINESE JOURNAL OF PHYSICS VOL. 49, NO. 1 FEBRUARY 2011 Laserinduced surface phonons and their excitation of nanostructures Markus Schmotz, 1, Dominik Gollmer, 1 Florian Habel, 1 Stephen Riedel, 1 and
More informationDoped Semiconductors. Dr. Katarzyna Skorupska
Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge
More informationRaman Scattering Theory David W. Hahn Department of Mechanical and Aerospace Engineering University of Florida (dwhahn@ufl.edu)
Introduction Raman Scattering Theory David W. Hahn Department of Mechanical and Aerospace Engineering University of Florida (dwhahn@ufl.edu) The scattering of light may be thought of as the redirection
More informationPhys 234H Practice Final Exam (Note: this practice exam contains more questions than will the final, which will have 25 multiplechoice questions.
Phys 234H Practice Final Exam (Note: this practice exam contains more questions than will the final, which will have 25 multiplechoice questions. MULTIPLE CHOICE. Choose the one alternative that best
More informationThe rate of change of velocity with respect to time. The average rate of change of distance/displacement with respect to time.
H2 PHYSICS DEFINITIONS LIST Scalar Vector Term Displacement, s Speed Velocity, v Acceleration, a Average speed/velocity Instantaneous Velocity Newton s First Law Newton s Second Law Newton s Third Law
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationFundamentals of Plasma Physics Waves in plasmas
Fundamentals of Plasma Physics Waves in plasmas APPLAuSE Instituto Superior Técnico Instituto de Plasmas e Fusão Nuclear Vasco Guerra 1 Waves in plasmas What can we study with the complete description
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationTime dependence in quantum mechanics Notes on Quantum Mechanics
Time dependence in quantum mechanics Notes on Quantum Mechanics http://quantum.bu.edu/notes/quantummechanics/timedependence.pdf Last updated Thursday, November 20, 2003 13:22:3705:00 Copyright 2003 Dan
More informationPHY4604 Introduction to Quantum Mechanics Fall 2004 Practice Test 3 November 22, 2004
PHY464 Introduction to Quantum Mechanics Fall 4 Practice Test 3 November, 4 These problems are similar but not identical to the actual test. One or two parts will actually show up.. Short answer. (a) Recall
More informationDO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS
DO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS Quantum Mechanics or wave mechanics is the best mathematical theory used today to describe and predict the behaviour of particles and waves.
More informationInfrared Spectroscopy: Theory
u Chapter 15 Infrared Spectroscopy: Theory An important tool of the organic chemist is Infrared Spectroscopy, or IR. IR spectra are acquired on a special instrument, called an IR spectrometer. IR is used
More informationSound. References: L.D. Landau & E.M. Lifshitz: Fluid Mechanics, Chapter VIII F. Shu: The Physics of Astrophysics, Vol. 2, Gas Dynamics, Chapter 8
References: Sound L.D. Landau & E.M. Lifshitz: Fluid Mechanics, Chapter VIII F. Shu: The Physics of Astrophysics, Vol., Gas Dynamics, Chapter 8 1 Speed of sound The phenomenon of sound waves is one that
More informationBlackbody radiation derivation of Planck s radiation low
Blackbody radiation derivation of Planck s radiation low 1 Classical theories of Lorentz and Debye: Lorentz (oscillator model): Electrons and ions of matter were treated as a simple harmonic oscillators
More informationCHEM344 HW#7 Due: Fri, Mar BEFORE CLASS!
CHEM344 HW#7 Due: Fri, Mar 14@2pm BEFORE CLASS! HW to be handed in: Atkins Chapter 8: Exercises: 8.11(b), 8.16(b), 8.19(b), Problems: 8.2, 8.4, 8.12, 8.34, Chapter 9: Exercises: 9.5(b), 9.7(b), Extra (do
More informationThe Kinetic Theory of Gases Sections Covered in the Text: Chapter 18
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
More informationGroup Theory and Chemistry
Group Theory and Chemistry Outline: Raman and infrared spectroscopy Symmetry operations Point Groups and Schoenflies symbols Function space and matrix representation Reducible and irreducible representation
More informationSection 3: Crystal Binding
Physics 97 Interatomic forces Section 3: rystal Binding Solids are stable structures, and therefore there exist interactions holding atoms in a crystal together. For example a crystal of sodium chloride
More informationChapter 18 4/14/11. Superposition Principle. Superposition and Interference. Superposition Example. Superposition and Standing Waves
Superposition Principle Chapter 18 Superposition and Standing Waves If two or more traveling waves are moving through a medium, the resultant value of the wave function at any point is the algebraic sum
More informationE. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE
E. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE References for Nuclear Magnetic Resonance 1. Slichter, Principles of Magnetic Resonance, Harper and Row, 1963. chapter
More informationLECTURE 11 : GLASSY DYNAMICS  Intermediate scattering function  Mean square displacement and beyond  Dynamic heterogeneities  Isoconfigurational
LECTURE 11 : GLASSY DYNAMICS  Intermediate scattering function  Mean square displacement and beyond  Dynamic heterogeneities  Isoconfigurational Ensemble  Energy landscapes A) INTERMEDIATE SCATTERING
More informationA.C. Conductivity and Dielectric Behaviour of Chalcogenide Ge x Fe x Se 1002x Thin Films.
Egypt. J. Sol., Vol. (25), No. (1), (2002) 49 A.C. Conductivity and Dielectric Behaviour of Chalcogenide Ge x Fe x Se 1002x Thin Films. M.I.Mohammed *, A.S.Abdrabo and E.A.Mahmoud *Physics department,
More informationThe nearlyfree electron model
Handout 3 The nearlyfree electron model 3.1 Introduction Having derived Bloch s theorem we are now at a stage where we can start introducing the concept of bandstructure. When someone refers to the bandstructure
More informationd d Φ * Φdx T(B) Barrier (B ) : Vo = 5, a = 2 Well (W ) : Vo= 5, a = 2 0.0 0 2 4 6 8 10 12 14 16 18 20 ENERGY (E)
Quantum Mechanical Transmission with Absorption S. MAHADEVAN, A. UMA MAHESWARI, P. PREMA AND C. S. SHASTRY Physics Department, Amrita Vishwa Vidyapeetham, Coimbatore 641105 ABSTRACT Transmission and reflection
More informationChapter 9 Summary and outlook
Chapter 9 Summary and outlook This thesis aimed to address two problems of plasma astrophysics: how are cosmic plasmas isotropized (A 1), and why does the equipartition of the magnetic field energy density
More information1.5 Light absorption by solids
1.5 Light absorption by solids BlochBrilloin model L e + + + + + allowed energy bands band gaps p x In a unidimensional approximation, electrons in a solid experience a periodic potential due to the positively
More informationFrom Fourier Series to Fourier Integral
From Fourier Series to Fourier Integral Fourier series for periodic functions Consider the space of doubly differentiable functions of one variable x defined within the interval x [ L/2, L/2]. In this
More informationPart 5: The BoseEinstein Distribution
PHYS393 Statistical Physics Part 5: The BoseEinstein Distribution Distinguishable and indistinguishable particles In the previous parts of this course, we derived the Boltzmann distribution, which described
More informationIntroduction to quantum mechanics
Introduction to quantum mechanics Lecture 3 MTX9100 Nanomaterjalid OUTLINE What is electron particle or wave?  How large is a potential well? What happens at nanoscale? What is inside? Matter Molecule
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationTheory of electrons and positrons
P AUL A. M. DIRAC Theory of electrons and positrons Nobel Lecture, December 12, 1933 Matter has been found by experimental physicists to be made up of small particles of various kinds, the particles of
More informationThe Central Equation
The Central Equation Mervyn Roy May 6, 015 1 Derivation of the central equation The single particle Schrödinger equation is, ( H E nk ψ nk = 0, ) ( + v s(r) E nk ψ nk = 0. (1) We can solve Eq. (1) at given
More informationA8 Thermal properties of materials
A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the
More informationSemiconductors Band Formation & direct and indirect gaps. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Semiconductors Band Formation & direct and indirect gaps 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/semi2013 Review of Energy Bands (1)
More informationMonte Carlo Simulation technique. S. B. Santra Department of Physics Indian Institute of Technology Guwahati
Monte Carlo Simulation technique S. B. Santra Department of Physics Indian Institute of Technology Guwahati What is Monte Carlo (MC)? Introduction Monte Carlo method is a common name for a wide variety
More information1 The water molecule and hydrogen bonds in water
The Physics and Chemistry of Water 1 The water molecule and hydrogen bonds in water Stoichiometric composition H 2 O the average lifetime of a molecule is 1 ms due to proton exchange (catalysed by acids
More informationSpectroscopy. The Interaction of Electromagnetic Radiation (Light) with Molecules
Spectroscopy. The Interaction of Electromagnetic Radiation (Light) with Molecules (1) Electromagnetic Radiationwave description propagation c = 3 x 10 10 cm/sec magnetic () and electric (E) field vectors
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationDamping in a variable mass on a spring pendulum
Damping in a variable mass on a spring pendulum Rafael M. Digilov, a M. Reiner, and Z. Weizman Department of Education in Technology and Science, TechnionIsrael Institute of Technology, Haifa 32000, Israel
More informationAnalysis of shear modes in a piezoelectric vibrator
JOURNAL OF APPLIED PHYSICS VOLUME 83, NUMBER 8 15 APRIL 1998 Analysis of shear modes in a piezoelectric vibrator Wenwu Cao, a) Shining Zhu, b) and Bei Jiang Materials Research Laboratory, The Pennsylvania
More information7. DYNAMIC LIGHT SCATTERING 7.1 First order temporal autocorrelation function.
7. DYNAMIC LIGHT SCATTERING 7. First order temporal autocorrelation function. Dynamic light scattering (DLS) studies the properties of inhomogeneous and dynamic media. A generic situation is illustrated
More informationBasic Principles of Magnetic Resonance
Basic Principles of Magnetic Resonance Contents: Jorge Jovicich jovicich@mit.edu I) Historical Background II) An MR experiment  Overview  Can we scan the subject?  The subject goes into the magnet 
More informationFourier Series. A Fourier series is an infinite series of the form. a + b n cos(nωx) +
Fourier Series A Fourier series is an infinite series of the form a b n cos(nωx) c n sin(nωx). Virtually any periodic function that arises in applications can be represented as the sum of a Fourier series.
More informationDynamic wave dispersion and loss properties of conventional and negative Poisson's ratio polymeric cellular materials 1 INTRODUCTION
Chen and Lakes 1 Dynamic wave dispersion and loss properties of conventional and negative Poisson's ratio polymeric cellular materials by C. P. Chen and R. S. Lakes Adapted from Cellular Polymers, 8, 343369,
More informationMaterial Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India
Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 5612 India Chapter 15. Thermal properties Engineering materials are important
More informationHeating & Cooling in Molecular Clouds
Lecture 8: Cloud Stability Heating & Cooling in Molecular Clouds Balance of heating and cooling processes helps to set the temperature in the gas. This then sets the minimum internal pressure in a core
More informationExperiment 1 Wave Phenomena: Interference
Experiment 1 Wave Phenomena: Interference 1. Objectives Observe the wavecharacteristic of light using diffraction and interference. Apply the law of diffraction to find the wavelength of the light and
More informationBondcorrelated percolation model and the unusual behaviour of supercooled water
J. Phys. A: Math. Gen. 16 (1983) L321L326. Printed in Great Britain LETTER TO THE EDITOR Bondcorrelated percolation model and the unusual behaviour of supercooled water ChinKun Hu LashMiller Chemical
More informationCLASSICAL CONCEPT REVIEW 8
CLASSICAL CONCEPT REVIEW 8 Kinetic Theory Information concerning the initial motions of each of the atoms of macroscopic systems is not accessible, nor do we have the computational capability even with
More informationNMR Techniques Applied to Mineral Oil, Water, and Ethanol
NMR Techniques Applied to Mineral Oil, Water, and Ethanol L. Bianchini and L. Coffey Physics Department, Brandeis University, MA, 02453 (Dated: February 24, 2010) Using a TeachSpin PS1A pulsed NMR device,
More informationLaminar and Turbulent flow. Flow Sensors. Reynolds Number. Thermal flow Sensor. Flow and Flow rate. R = Mass Flow controllers
Flow and Flow rate. Laminar and Turbulent flow Laminar flow: smooth, orderly and regular Mechanical sensors have inertia, which can integrate out small variations due to turbulence Turbulent flow: chaotic
More informationUniversity of Toronto Department of Electrical and Computer Engineering. ECE 330F SEMICONDUCTOR PHYSICS Eng. Annex 305
University of Toronto Department of Electrical and Computer Engineering ECE 330F SEMICONDUCTOR PHYSICS Eng. Annex 305 Experiment # 1 RESISTIVITY AND BAND GAP OF GERMANIUM TA: Iraklis Nikolalakos OBJECTIVE
More information21 The Nature of Electromagnetic Waves
21 The Nature of Electromagnetic Waves When we left off talking about the following circuit: I E v = c B we had recently closed the switch and the wire was creating a magnetic field which was expanding
More informationAP1 Oscillations. 1. Which of the following statements about a springblock oscillator in simple harmonic motion about its equilibrium point is false?
1. Which of the following statements about a springblock oscillator in simple harmonic motion about its equilibrium point is false? (A) The displacement is directly related to the acceleration. (B) The
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationSpectroscopic Notation
Spectroscopic Notation Most of the information we have about the universe comes to us via emission lines. However, before we can begin to understand how emission lines are formed and what they tell us,
More informationF en = mω 0 2 x. We should regard this as a model of the response of an atom, rather than a classical model of the atom itself.
The Electron Oscillator/Lorentz Atom Consider a simple model of a classical atom, in which the electron is harmonically bound to the nucleus n x e F en = mω 0 2 x origin resonance frequency Note: We should
More informationPhysics 551: Solid State Physics F. J. Himpsel
Physics 551: Solid State Physics F. J. Himpsel Background Most of the objects around us are in the solid state. Today s technology relies heavily on new materials, electronics is predominantly solid state.
More informationSize effects. Lecture 6 OUTLINE
Size effects 1 MTX9100 Nanomaterials Lecture 6 OUTLINE Why does size influence the material s properties? How does size influence the material s performance? Why are properties of nanoscale objects
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More information develop a theory that describes the wave properties of particles correctly
Quantum Mechanics Bohr's model: BUT: In 192526: by 1930s:  one of the first ones to use idea of matter waves to solve a problem  gives good explanation of spectrum of single electron atoms, like hydrogen
More informationThermal Properties of Matter
Chapter 18 Thermal Properties of Matter PowerPoint Lectures for University Physics, Thirteenth Edition Hugh D. Young and Roger A. Freedman Lectures by Wayne Anderson Goals for Chapter 18 To relate the
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More information